Date post: | 04-Apr-2015 |

Category: |
## Documents |

Upload: | alejandro-del-paso |

View: | 151 times |

Download: | 7 times |

Share this document with a friend

12

Transcript

2 PHYSICAL BASIS

2.1 The piezoelectric effect in ceramic materials

The piezoelectric effect was discovered by Jacques andPierre Curie in 1880. They found that if certain crystalswere subjected to mechanical strain, they became electri-cally polarized and the degree of polarization was propor-tional to the applied strain. The Curies also discoveredthat these same materials deformed when they wereexposed to an electric field. This has become known asthe inverse piezoelectric effect.

The piezoelectric effect is exhibited by a number ofnaturally-occurring crystals, for instance quartz,tourmaline and sodium potassium tartrate, and these havebeen used for many years as electromechanicaltransducers. For a crystal to exhibit the piezoelectriceffect, its structure should have no centre of symmetry. Astress (tensile or compressive) applied to such a crystalwill alter the separation between the positive andnegative charge sites in each elementary cell leading to anet polarization at the crystal surface. The effect ispractically linear, i.e. the polarization varies directly withthe applied stress, and direction-dependent, so thatcompressive and tensile stresses will generate electricfields and hence voltages of opposite polarity. It's alsoreciprocal, so that if the crystal is exposed to an electricfield, it will experience an elastic strain causing itslength to increase or decrease according to the fieldpolarity.

2.2 Piezoelectric materials

Besides the crystals mentioned above, an important groupof piezoelectric materials are the piezoelectric ceramics,of which PZT is an example. These are polycrystallineferroelectric materials with the perovskite crystalstructure - a tetragonal/rhombahedral structure very closeto cubic. They have the general formula A2+B1+02-

3, inwhich A denotes a large divalent metal ion such asbarium or lead, and B denotes a tetravalent metal ionsuch as titanium or zirconium. It's these materials that arethe subject of the present book (Ref. I ).

Materials such as PZT can be considered as a mass ofminute crystallites. Above a temperature known as theCurie point, these crystallites exhibit simple cubic sym-metry, the elementary cell of which is shown inFlg.2.1(a). This structure is centrosymmetric withpositive and negative charge sites coinciding, so there areno dipoles present in the material (which is said toexhibit paraelectric behaviour). Below the Curie point,however, the crystallites take on tetragonal symmetry inwhich the positive and negative charge sites no longercoincide (Fi2.2(b)), so each elementary cell then has abuilt-in electric dipole which may be reversed, and alsoswitched to certain allowed directions by the applicationof an electric field. Such materials are termedferroelectric because this electrical

behaviour presents a physical analogy with the magneticbehaviour of ferromagnetic materials. They don't neces-sarily contain iron as an important constituent. Theanalogy can, in fact, be carried further, since to someextent the polarization of ferroelectric materials exhibitshysteresis, and their dielectric constants are very highand temperature-dependent (as are the permeabilities offerromagnetic materials).

The dipoles are not randomly oriented throughout thematerial. Neighbouring dipoles align with each otherto form regions of local alignment known as Weissdomains. Within a Weiss domain, therefore, all thedipoles are aligned, giving a net dipole moment to thedomain, and hence a net polarization (dipole momentper unit volume).

Fig.2.1 PZT elementary cell.

(a) cubic lattice (above Curie temperature);

(b) tetragonal lattice (below Curie temperature)

alejandrodelpaso

Highlight

alejandrodelpaso

Highlight

alejandrodelpaso

Highlight

alejandrodelpaso

Highlight

alejandrodelpaso

Highlight

alejandrodelpaso

Highlight

Fig.2.2 Electric dipole moments in Weiss domains.(a) before polarization;(b) during polarization;(c) after polarization

The direction of polarization between neighbouringWeiss domains within a crystallite can differ by 90° or180°, and owing to the random distribution of Weissdomains throughout the material (Fig.2.2(a)), no overallpolarization or piezoelectric effect is exhibited.The ceramic may be made piezoelectric in any chosendirection by a poling treatment which involves exposing itto a strong electric field at a temperature slightly belowthe Curie point (Fig.2.2(b)). Under the action of this field,domains most nearly aligned with the field will grow atthe expense of other domains. The material will alsolengthen in the direction of the field. When the field isremoved (Fig.2.2(c)), the dipoles remain locked inapproximate alignment, giving the ceramic material aremanent polarization and a permanent deformation (i.e.making it anisotropic). The poling treatment is usually thefinal treatment of PZT component manufacture.

2.3 Dielectric hvsteresis

The electric field E and the polarization P are connected ina dielectric medium by the relation:

D - ε()E + P (2.1) in which ε() is the permittivity of free space and D is theelectric displacement. For a ferroelectric material likePZT, however, P is itself a function of E as shown inFig.2.3. In this figure, the hysteresis effect, familiar fromferromagnetics, is quite evident. If an initially unpolarizedsample of PZT is subjected to an increasing electric fieldat a temperature slightly below its Curie point, the dipolesbecome increasing aligned with the field and the polariz-ation will follow the `initial curve' shown in Fig.2.3.When the field has increased beyond a certain value, nofurther increase in polarization will be observed becausethe dipoles are then all aligned with the field. Thematerial is then said to have reached its saturationpolarization Ps*

If the field is now reduced to zero, the dipoles become lessstrongly aligned, since in the absence of an external fieldthey're bound to certain preferred directions within theindividual crystallites. They do not, however, return to theiroriginal alignment (i.e. the alignment before the field wasapplied) since there are several preferred directions within thecrystallites and the dipoles remain in the ones most closelyaligned with the original field. Since there is still, therefore, avery high degree of alignment (as can be seen from Fig.2.2(c)),the polarization does not fall back to zero but to a valuesomewhat lower than the saturation polarization known as theremanent polarization Pr

If the field is now increased in the opposite direction, thepolarization of the sample initially falls to zero and thenincreases in the negative direction until it reaches a saturationpolarization -Ps* If the field is again reduced to zero, thepolarization falls to the remanent polarization -Pr and finally, ifthe field is increased in the positive direction again, thepolarization will fall to zero and then eventually return to Ps*

The curve thus traced out is known as the hvsteresis curve.Its shape varies for the different PZT materials (Fig.2.3 is thehysteresis curve for a ‘soft’ PZT) but the remanent polarizationis generally around 0.3 C/m2 for all PZT materials.

The variation of electric displacement D as a function ofelectric field strength follows very closely the curve forpolarization. For example, at the peak of the hysteresiscurve (E - 1.6 kV/mm), D is only around 0.014 C/m2 higherthan P. At E = 0, D and P are equal, i.e. D, Pr

The lower part of Fig.2.3 shows the variation of thesample's relative extension S3 (i.e. in the direction ofpolarization) with electric field, and it can be seen that this alsoexhibits a hysteresis effect corresponding precisely with theeffect observed for polarization.

alejandrodelpaso

Highlight

alejandrodelpaso

Highlight

alejandrodelpaso

Highlight

Fig.2.3 Upper part of figure: dielectric hysteresis of a‘soft’ PZT. The electric displacement D(E) is obtained by

addition of EOE to the polarization P(E) in accordancewith Eq.2.1. Lower part of figure: mechanical

deformation S3 in the direction of polarization and field,as well as S1 and SL normal to this direction as a

function of field strength for a ‘soft’ PZT. The S1 curveis based on measurement, S3 is given by S3 -2S1 : -2S2

Since the volume of the sample remains roughlyconstant, a relative increase (or decrease) in S3 will beaccompanied by a relative decrease (or increase) in thesample's dimension perpendicular to the field (S1 and S2)equal to about half the change in S3 (the left hand scalein the lower part of Fig.2.3). This is also true,incidentally, for compressive and tensile forces exertedby the sample.

Finally, Fig.2.4 shows how S1 varies with electricdisplacement, and again shows the hysteresis effect.

Fig.2.4 Mechanical deformation (strain) S1 and S2 normal todirection of polarization as a function of electric

displacement for a ‘soft’ PZT

2.4 Basic behaviour of a piezoelectric ceramic body

Figure 2.5 illustrates the behaviour of a PZT cylinderpolarized along its axis. For clarity, the magnitude ofthe effect has been exaggerated.

Figure 2.5(a) shows the cylinder under no-loadconditions. If an external force produces compressiveor tensile strain in the material, the resulting change indipole moment causes a voltage to appear between theelectrodes. If the cylinder is compressed so that itresumes its original form, i.e. before poling, thevoltage will have the same polarity as the polingvoltage (Fig.2.5(b)). If it is stretched, the voltageacross the electrodes will have opposite polarity to thepoling voltage (Fig.2.5(c)). These are examples ofgenerator action: the conversion of mechanical energyinto electrical energy. Examples of piezoelectricinduced generator action can be found in cigarette andgas lighters, gramophone pick-ups, accelerometers,hydrophones and microphones.

If a voltage of opposite polarity to the polingvoltage in applied to the electrodes, the cylinder willshorten (Fig.2.5(d)). If the applied voltage has the samepolarity as the poling voltage, the cylinder willlengthen (Fig.2.5(e)).

Fig.2.5 The piezoelectric effect ina cylindrical body of piezoelectricceramic. For the sake of clarity,only a dipole has been drawn ineach case.For further details see text

Finally, if an alternating voltage is applied to the elec-trodes, the cylinder will grow and shrink at the samefrequency as that of the applied voltage (Fig.2.5(f)). Theseare examples of motor action: conversion of electricalenergy into mechanical energy.

Fig2.6 Decrease of coupling factor (kp) as a function of timefor a number of PXE grades

2.5 Stability

The properties of piezoelectric elements are more or lesstemperature dependent and time dependent. The stabilityas a function of time is of particular interest. Fortunatelythe poling ages approximately logarithmically so that therate of change in permittivity, coupling factor, frequencyconstant and so on (Section 2.11 ), decreases rapidly in thecourse of time. Powerful ambient influences are likely tochange the original ageing pattern. This appliesparticularly to the permittivity, the mechanical Qfactorand the dielectric loss factor tanδ.

2.6 Depolarization

As already mentioned, after its poling treatment a PZTceramic will be permanently polarized, and care musttherefore be taken in all subsequent handling to ensurethat the ceramic is not depolarized, since this will result inpartial or even total loss of its piezoelectric properties.The ceramic may be depolarized electrically, mechanicallyor thermally.

2.6.1 Electrical depolarization

Exposure to a strong electric field of opposite polarity tothe poling field will depolarize a piezoelectric element.The field strength required for marked depolarizationdepends, among other things, on the material grade, thetime the material is subjected to the depolarizing field andthe temperature. For static fields, it's typically between200 and 500 V/mm.

An alternating field will also have a depolarizingeffect during the half cycles that it opposes the polingfield.

2.6.2 Mechanical depolarizationMechanical depolarization occurs when the

mechanical stress on a piezoelectric element becomeshigh enough to disturb the orientation of the domainsand hence destroy the alignment of the dipoles. Thesafety limits for mechanical stress vary considerablywith material grade.

2.6.3 Thermal depolarizationIf a piezoelectric element is heated to its Curie point,the domains become disordered and the elementbecomes completely depolarized. A piezoelectricelement can therefore function for long period withoutmarked depolarization only at temperatures wellbelow the Curie point. A safe operating temperaturewould normally be about half way between 0 °C andthe Curie point.

2.7 Piezoelectric constantsSince piezoelectric ceramics are anisotropic, theirphysical constants (elasticity, permittivity etc.) aretensor quantities and relate to both the direction of theapplied stress, electric field etc., and to the directionsperpendicular to these. For this reason the constantsare generally given two subscript indices which referto the direction of the two related quantities (e.g.stress and strain for elasticity, displacement andelectric field for permittivity). A superscript index isused to indicate a quantity that's kept constant (Ref.2).

The direction of positive polarization is usuallychosen to coincide with the Z-axis of a rectangularsystem of crystalographic axes X, Y, Z. If thedirections of X, Y and

Z are represented by 1, 2 and 3 respectively, andthe shear about these axes by 4, 5 and 6 respectively,the various constants may be written with subscriptsreferring to these (Fig.2.7).

alejandrodelpaso

Highlight

alejandrodelpaso

Highlight

Permittivity EThe (absolute) permittivity (or dielectric constant) isdefined as the dielectric displacement per unit electricfield. The first subscript gives the direction of thedielectric displacement, the second gives the directionof the electric field. For example:

The tables in our Data handbook give values for therelative permittivity c/e, i.e. the ratio of absolutepermittivity to the permittivity of free space (8.85 x10 -12 F/m).

Compliance sThe compliance s of a material is defined as the strainproduced per unit stress. It's the reciprocal of the modulusof elasticity. The first subscript refers to the direction ofstrain, the second to direction of stress. For example:

Piezoelectric charge constants dThe piezoelectric charge constant is defined as theelectric polarization generated in a material per unitmechanical stress applied to it. Alternatively, it is themechanical strain experienced by the material per unitelectric field applied to it. The first subscript refers tothe direction of polarization generated in the material(at E = 0) or to the applied field strength, the secondrefers respectively to the direction of the applied stressor to the direction of the induced strain. For example:

Piezoelectric voltage constant gThe piezoelectric voltage constant is defined as theelectric field generated in a material per unit mechanicalstress applied to it. Alternatively, it is the mechanicalstrain experienced by the material per unit electricdisplacement applied to it. The first subscript refers to thedirection of the electric field generated in the material orto the applied electric displacement, the second refersrespectively to the direction of the applied stress or to thedirection of the induced strain. For example:

2.8 ExamplesTo give an indication of the stresses, strains, voltages etc.that accompany piezoelectric transducer action, let'sconsider the example of a piezoelectric cylinder 20 mmlong and I cm2 in cross-section subject to an externalstress. This is an example of generator action, i.e. theconversion of mechanical energy into electrical energy.Provided the ends of the cylinder are not connectedtogether, no current flows and the dielectric displacementD is zero.

Figure 2.8 shows that the open-circuit voltage V(and hence the field strength E) is proportional tocompressive stress T up to a maximum of 25 kV, whichoccurs at a stress of 50 MPa1) (see Eq.A in theAppendix).1) 1 0 6 N / m 2

This can be expressed as:

or, since V = El and T - F/A,

in which F is the force applied to the ends of thecylinder of cross section A and length l, and g is thepiezoelectric voltage constant defined in Section 2.7(dimension m 2/C or Vm/N). Note: by definition, thevoltage or electric field generated is said to bepositive if it's polarity is the same as that of theoriginal poling voltage.

With g - d/ET (see Appendix, Eq.A), Eq.2.3a can berewritten as:

In which C is the capacitance of the piezoelectriccylinder and ET is the dielectric constant at (constant)pressure T. So the charge Q = CV on the cylinder(compare Fig.2.8(b)) is given by:

The induced charge therefore is completely independentof cylinder dimensions and hence of its tolerances (incontrast to the induced voltage). In this example, theinduced charge is about 2 pC, but this depends heavily ontemperature since g and ET are temperature dependent(with temperature coefficients of opposite sign).

Stresses of 50 MPa are easily obtained with simplepresses. Even the bare hand can produce forces of sometens of newtons, and it only takes about 25 N to generate100 V with the above cylinder. The electrical energy thisgenerates, however, is far too low to be hazardous.

Examples where mechanical energy (movement) isconverted into electrical energy or into an electrical signalinclude: gas cigarette lighters and various domestic gas-ignition devices, gramophone pickups, accelerometers,microphones and hydrophones.

The conversion of electrical energy into mechanicalmovement is governed by the equation (corresponding toequation A in the appendix):

in which S is the mechanical strain (Fig.2.9) generated byelectric field E or voltage V across the cylinder. Thedimensions of the piezoelectric charge constant d are C/Nor m/V. Since S Ol/I

from which we can deduce that A/ is independent of thedimensions of the PZT cylinder. For a PZT 5A cylindersubject to 16 kV (E - 800 V/m), Al equals about 10 ftm.

Fig.2.9 Pressure exerted on the cylinder generates.

(a) voltage V which depends on length l and cross-section A of the cylinder;

(b) charge which is completely independent of thecylinder dimensions;

(c) voltage applied to the PZT cylinder leads to arelative change in length S1 which depends onthe length I of the cylinder, and an absolutechange in length p independent of cylinderdimensions

The figures quoted here refer to static loads; analternating field generally yields different results. Inparticular, at the mechanical resonant frequency, theamplitude of oscillation can be expected to be muchgreater than the static changes. For relatively largemechanical movement (> 1 mm say) special flexionalelements are available.

Examples where electrical energy is converted intomechanical energy can be found in atomizers andequipment for ultrasonic cleaning, welding, solderingand ultrasonic drilling.

2.9 Dynamic behaviour of PZT transducersWhen exposed to an alternating electric field, a piezo-electric element periodically changes its size inaccordance with the frequency of the field. In otherwords it oscillates and, if the frequency lies in thevicinity of its series resonant frequency (see below fordefinition) its behaviour can be described by theequivalent circuit of Fig.2.10.

Fig.2.10 Equivalent circuit diagram of a PZT transducer.C0 is the capacitance of the transducer below the resonant

frequency minus capacitance C1 ,R1 is the resistance caused by mechanical lossesRL the resistance of the working load due to the radiated

energy: in vacuum RL = 0,C1 the capacitance of the mechanical circuit and L1 is the

inductance of the mechanical circuit

For such an oscillating system, Fig.2.ll shows the variation ofadmittance Y and impedance Z with frequency. The frequency fm atwhich the admittance becomes maximum (minimum impedancefrequency) lies close to the series resonant frequency

(The frequency at which the impedance in the equivalent circuitbecomes zero when R1 is neglected).

The frequency fn at which the admittance becomes minimum (maximumimpedance frequency) lies close to the parallel resonant frequency

(The frequency at which the parallel resistance in the equivalent circuitbecomes infinite, again neglecting R1).

Fig.2.11 Admittance and impedance as functionsof frequency. The series resonant frequency fs lies inthe vicinity of the minimum impedance frequencyfm the parallel resonant frequency fp lies inthe vicinity of the maximum impedancefrequency fn Below fm and above fn the transducerbehaves capacitively, between fm and fn it behavesinductively

Fig.2.12 Equivalent circuits for tuned

Fig.2.13 Impedance curves for tuned transducers

It's often advisable to tune the transducer with a seriesor parallel inductance, Lpar or Lser given by:

In this way, two coupled resonant circuits are obtained: onemechanical, governed by L1, C1 and R1, the other electrical,governed by Lpar (or Lser), C() and the resistor R of the ACvoltage generator. The frequency response of such a coupledsystem resembles that of a band-pass filter.

Figure 2.12 shows the equivalent circuit for a tunedsystem (series and parallel tuning) and Fig.2.13 shows the

variation of impedance with frequency. Curve I applies to anacoustically unloaded oscillator, curves II or III to anoscillator in which the loading is average or strong.

The impedance of the parallel-tuned system at fs, is real,and that of the series-tuned system is real at fp. Although thefrequency-response curve depends to some extent on theelectrical termination resistance and mechanical load, theeffect on bandwidth B, and on fs. and fp is not great. Thebandwidth obtained by electrical tuning is roughly theproduct of the effective coupling coefficient keff (see. section2.11) and the series or parallel resonant frequency, i.e

B = keff fsp (2.1 I)

2.10 Frequency constant N

The resonant frequencies referred to in the previoussection depend, of course, on the dimensions of the PZTsample, and experience indicates that they vary inverselywith these dimensions. Figure 2.14, for example, showsthe variation of impedance with frequency for a PZT5Adisc, I mm thick and 25 mm in diameter. An impedance-minimum occurs at a series-resonant frequency fs of

Fig.2.14 Measured impedance of a PZT5A disc (dimensions 25mm 0 x 1 mm) in the region of planar resonance

Known as the planar or radial resonant frequency, it's relatedto the disc diameter D by

NEP, which for PZT5A material equals 2000 m/s is known as

the planar or radial frequency constant.

Figure 2.15 is similar to Fig.2.14 but with the frequencyscale extended to 3 MHz to show higher resonances. Theimpedance minimum at about 2 MHz is known as the axialresonance, and its frequency is related to the thickness h ofthe disc by

ND3 is known as the thickness frequency constant and for

PZT5A material it equals 1850 m/s (≈1 x 10-3 m x 2 x 106

Hz).So the frequency constant is the product of the series

resonant frequency fs and the dimensions governing thatfrequency. The subscript indicates the type of oscillation atresonance: p for planar oscillations, 3 for oscillations in theZ or axial direction.

Fig.2.15 Measured impedance of a PZT5A disc (dimensions 25mm ∅ x 1 mm) in the region up to 3 MHz. The planarresonance and thickness resonance are clearly recognizable.For further information see text.

Frequency constants are always quoted in our data sheetsand data handbook (MA03) on PZT materials, so using theabove relations, it's an easy matter to calculate the seriesresonant frequency of a PZT oscillator. The frequencyconstant can, in fact, he shown to equal half the soundvelocity in the ceramic material (with the exception of Np).

Figures 2.14 and 2.15 relate to freely oscillating PZTbodies. Behaviour changes quite dramatically if the bodiesare constrained. Figure 2.16, for example, shows how theimpedance of a diaphragm on which a PZT disc is gluedvaries with frequency (for details see caption to figure).

Fig.2.16 Impedance as a function of the frequency of afreely oscillating diaphragm

(dimensions 43 mm ∅ x 0.15 mm) on to which a PZT5A disc(dimensions 25 mm ∅ x 0.15 mm) has been glued

2.11 Coupling factor kAnother important constant for piezoelectric materials isthe coupling factor k e f f which is a measure of the effec-tiveness with which electrical energy in converted intomechanical energy and vice versa. At frequencies wellbelow the resonant frequency of the piezoelectric body,keff is given by the expression

(see appendix for derivation).This expression holds for both electromechanical

and mechano-electrical conversions.A study of the values of keff shows that for modernpiezoelectric ceramics, up to 509 of the stored energycan be converted at low frequencies. The values of k2

effquoted in tables, however, are usually theoreticalmaxima, based on precisely defined vibrational modes ofideal (i.e. unrealistic) specimens of the material. Inpractical transducers, the coupling factors are usuallylower.As with other piezoelectric constants, coupling factorscarry subscripts. k33, for instance, is the coupling factorfor longitudinal vibrations of a very long, very slenderrod (in theory infinitely long, in practice, with alength/diameter ratio > 10) under the influence of alongitudinal electric field. k31 is the coupling factor forlongitudinal vibrations of long rod under the influenceof a transverse electric field, and kl5 describes shearmode vibrations of a piezoelectric body.

Special cases of the coupling factor are the planarcoupling factor k/, and the thickness coupling factor kr.The planar coupling factor kp of a thin disc representsthe coupling between the electric field in direction 3(parallel to the disc axis) and simultaneous mechanicaleffects in directions 1 and 2 (Fig.2.17) that result inradial vibrations. This is known as radial coupling.

The thickness coupling factor kf represents thecoupling between an electric field in direction 3 andthe mechanical vibrations in direction 3 of a -thin,planar object of arbitrary contour (i.e. an object whosesurface dimensions are large compared with itsthickness).

The resonant frequency of the thickness mode of athin planar object is far higher than that of itstransverse mode.

Fig.2.17 Planar oscillations of a thin discof piezoelectric material

What's more, since its overall volume remainssubstantially constant, expansion/contraction inthickness must always be accompanied bycorresponding contraction/expansion in the transversedirections, so the strongly attenuated transversevibrations at the higher resonant frequency of thethickness mode tend to increase the apparent stiffnessof the material. Hence k t is lower than k 33 - thecoupling factor for longitudinal vibrations of a slenderrod (whose longitudinal resonant frequency is muchlower and matches more closely its transverse resonantfrequency).

Although a high k 2e f f is usually desirable for

efficient transduction, it should not be thought of as ameasure of efficiency, since the unconverted energy isnot necessarily lost (converted into heat) and can inmany cases be recovered.

The real efficiency is the ratio of the converteduseful energy to the energy taken up by the transducer,and a tuned and well-adjusted transducer working in itsresonance region could be more than 90% efficient.Well outside its resonance region, however, itsefficiency could be very low.

2.12 Comparison of piezoelectric ceramicand crystalline quartz

This section details some of the importantdifferences between PZT and crystalline quartz,differences that in many instances account for their usein quite widely differing application areas. As we saidearlier, the ferroelectric properties of PZT mean that ishas a very much higher dielectric constant than quartz(see Table I ). Likewise, the coupling factor andpiezoelectric charge constant of PZT are considerablyhigher than those of quartz, and hence volume-for-volume, its performance as a transducer is far superiorto that of quartz, allowing expensive amplifiers to bedispensed with.

On the other hand, quartz has a Q factor severaltimes higher than that of PZT.

TABLE 1Some piezoelectric materials

Symbol Unit QuartzPZT5A(NavyII

)PZT4(Nav

y I)

DielectricConstant εT

33/ε() 4.5 1800 1300

CouplingFactor K33 0.09 0.66 0.60

ChargeConstant D33 10-12C/N 2.0 460 300

VoltageConstant G33 10-3 Vm/N -50 28 25

QualityFactor Q 104-106 80 600

For significance of indices see section 2 6

These differences in material properties naturallylead to PZT and quartz being used in differentapplication areas. Quartz, for example, is ideal forhigh-Q, high precision mechanical resonators, asused for frequency stabilizers in clocks and watches.

PZT materials, on the other hand, are less popularas resonators, their main application areas being in,for example, actuating systems (stacked elements) inwhich they operate well below their naturalresonances and in which the ability to generate highforce or large displacements is more important. Inother applications (for example high-performanceultrasonic transducers), high conversion efficiencyand design versatility are important, and here PZT isideal thanks to the ease with which it can befashioned into almost any shape, and, in contrast toquartz, its ability to be polarized in any desireddirection.

2.13 Pyroelectric effectsThe polarization in piezoelectric materials is

temperature dependent. The oriented structure of theelectric dipoles gradually disappears with risingtemperature. Within the safe operating temperaturerange the changes are reversible. When exposed toexcessive heat permanent loss of polarization willoccur. Changes in the alignment of the dipoles leadto charge displacements and electric fields.

In most applications this phenomenon is anunwanted side-effect which causes measuring errorsor even failure of sensitive electronic componentslike MOSFETS by overvoltage.

In other applications the effect is very useful, forinstance in infrared detectors.Infrared radiation heats up the ceramic, the resultingvoltage or charge is a measure for the level of theradiation.In most cases however it is a nuisance. Theinterference mainly occurs in very low frequency orquasi-static applications. To suppress it parallelresistors are used to allow the charge to flow away. Insensors this causes an unwanted uplift of the lowercut-off frequency. In this section a qualitative as wellas a quantitative overview of the pyroelectric effectwill be given.

A measure for the effect are the so-calledpyroelectric coefficients dP/dT and dE/dT.

For our PZT range the following values are typical:

Fig.2.19 and 2.20 show the results of measurements onPZT5A discs.

Room temperature was taken as a reference andtemperature cycles were carried out at a rate of 3K/min. When a specimen is heated to 100 °C for thefirst time a considerable irreversible change inpolarization takes place. After a few cycles thechanges become almost purely reversible.

Fig.2.19 The polarization of PZT5A during temperature cycling

From Fig.2.20(a) it is clear that ∆ P is almost alinear function of temperature. The curve for ∆ Ehowever deviates from being linear because thedielectric constant (E) is also a function oftemperature.

The following example clearly demonstrates theimportance and danger of the pyroelectric effect:

∆ T = 10KPZT5A disc of ∅10 x I mm.A E = 20 x 103 V/(mK) x 10 K -- 200 x 103 V/m∆ V = ∆ E . h = 2 0 0 x 1 0 3V/m x 103m=200V.

Clearly this voltage would destroy a MOSFETamplifier stage immediately.

Figure 2.21 shows measured values of (dP)/(dT)as a function of temperature for several PZT materialgrades. The average of all curves confirms the valueof 400 x 10-6 C/(m2K) mentioned before. Theliberated pyroelectric charge for a temperaturechange can be calculated with the formula:

where A is the surface area of the PZT-element.

Fig.2.20 The pyroelectric voltage effect of PZT5A

Given a possible rate of temperature change, theleakage resistor necessary to keep the interferencewithin limits can now be calculated. In criticalapplications material grades with the highest ratiobetween piezoelectric (d33) and pyroelectric chargeconstant (dP/dT) should be used. PZT5A is the bastgrade in this respect.

Figure 2.22 provides information about thepyroelectric constants of field-strength (dEldT) forthe range of PZT grades. These constants areimportant to predict their behaviour under opencircuit conditions, as is the case in spark generatorsand often in accelleration sensors.

The generated pyroelectric voltage is given by:

h - height of PZT-element

In this case a measure for material quality is the ratiobetween the piezoelectric voltage constant (g33) and thepyroelectric field strength constant (dE/dT).

.

Fig.2.21 Pyroelectric charge constant forseveral PZT grades

Fig.2.22 Pyroelectric voltage constant forseveral PZT grades

PZT4(NavyI)PZT5A(NavyII)

PZT8(NavyIII)

Delete lines for 41, 21 & 71

Repeat as above renaming 5, 42and 43. Delete 21, 71 and 41

Recommended